# POURING THE MOLTEN METAL

Save this PDF as:

Size: px
Start display at page:

## Transcription

1 HEATING AND POURING To perform a casting operation, the metal must be heated to a temperature somewhat above its melting point and then poured into the mold cavity to solidify. In this section, we consider several aspects of these two steps in casting. Heating furnaces of various kinds are used to heat the metal to a molten temperature sufficient for casting. The heat energy required is the sum of (1) the heat to raise the temperature to the melting point, (2) the heat of fusion to convert it from solid to liquid, (3) the heat to raise the molten metal to the desired temperature for pouring. This can be expressed: H= ρv{cs[t m -T o ]+ H f + C l (Tp-Tm)} Where H= total heat required to raise the temperature of the metal to the pouring temperature, J ρ=density g/cm 3 V= Volume of metal Heated cm 3 H f = Heat of Fusion J/g Cs= weight specific heat for the solid metal, J/g C Cl= weight specific heat of the liquid metal, J/g C Tp= Pouring Temperature C Tm=Melting Temperature of metal C T o = starting temperature-usually ambient- C The above equation is of conceptual value, but its computational value is limited, notwithstanding our example calculation. Use of Eq. (1) is complicated by the following factors: (1) Specific heat and other thermal properties of a solid metal vary with temperature, especially if the metal undergoes a change of phase during heating. (2)A metal s specific heat may be different in the solid and liquid states.

2 (3) Most casting metals are alloys, and most alloys melt over a temperature range between a solidus and liquidus rather than at a single melting point; thus, the heat of fusion cannot be applied so simply as indicated above. (4) The property values required in the equation for a particular alloy are not readily available inmost cases. (5) There are significant heat losses to the environment during heating. EX1 One cubic meter of a certain eutectic alloy is heated in a crucible from room temperature to 100 C above its melting point for casting. The alloy s density = 7.5 g/cm3, melting point = 800 C, specific heat=0.33 J/g C in the solid state and 0.29 J/g C in the liquid state; and heat of fusion= 160 J/g. How much heat energy must be added to accomplish the heating, assuming no losses? Sol: (( 0.29( ( 25)+ )}(0:33)(800-6 {7.5(10 = H =3335(10 6 ) J

3 POURING THE MOLTEN METAL After heating, the metal is ready for pouring. Introduction of molten metal into the mold, including its flow through the gating system and into the cavity, is a critical step in the casting process. For this step to be successful, the metal must flow into all regions of the mold before solidifying. Factors affecting the pouring operation include pouring temperature, pouring rate, and turbulence The pouring temperature is the temperature of the molten metal as it is introduced into the mold. What is important here is the difference between the temperature at pouring and the temperature at which freezing begins (the melting point for a pure metal or the liquidus temperature for an alloy). This temperature difference is sometimes referred to as the superheat. This term is also used for the amount of heat that must be removed from the molten metal between pouring and when solidification commences. Pouring rate refers to the volumetric rate at which the molten metal is poured into the mold. If the rate is too slow, the metal will chill and freeze before filling the cavity. If the pouring rate is excessive, turbulence can become a serious problem. Turbulence in fluid flow is characterized by erratic variations in the magnitude and direction of the velocity throughout the fluid. The flow is agitated and irregular rather than smooth and streamlined, as in laminar flow. Turbulent flow should be avoided during pouring for several reasons. It tends to accelerate the formation of metal oxides that can become entrapped during solidification, thus degrading the quality of the casting. Turbulence also aggravates mold erosion, the gradual wearing away of the mold surfaces due to impact of the flowing molten metal. The densities of most molten metals are much higher than water and other fluids we normally deal with. These molten metals are also much more chemically reactive than at room temperature. Consequently, the wear caused by the flow of these metals in the mold is significant, especially under turbulent conditions. Erosion is especially serious when it

4 occurs in the main cavity because the geometry of the cast part is affected. ENGINEERING ANALYSIS OF POURING There are several relationships that govern the flow of liquid metal through the gating system and into the mold. An important relationship is Bernoulli s theorem, which states that the sum of the energies (head, pressure, kinetic, and friction) at any two points in a flowing liquid are equal. This can be written in the following form : h 1 + P 1 ρ = v 2 1 2g + F 1 = P 2 ρ + v 2 2 2g + F 2 Bernoulli s equation can be simplified in several ways. If we ignore friction losses (to be sure, friction will affect the liquid flow through a sand mold), and assume that the system remains at atmospheric pressure throughout, then the equation can be reduced to h 1 + v 1 2 2g = h 2 + v 2 2 2g This can be used to determine the velocity of the molten metal at the base of the sprue. Let us define point 1 at the top of the sprue and point 2 at its base. If point 2 is used as the reference plane, then the head at that point is zero (h 2 = 0) and h 1 is the height (length) of the sprue. When the metal is poured into the pouring cup and overflows down the sprue, its initial velocity at the top is zero (v1 = 0). Hence, Eq. (3) further simplifies to h 1 = v 2 2 2g which can be solved for the flow velocity

5 v = 2gh 2 where v=the velocity of the liquid metal at the base of the sprue, cm/s; g=981 cm/s/s and h = the height of the sprue, cm Another relationship of importance during pouring is the continuity law, which states that the volume rate of flow remains constant throughout the liquid. The volume flow rate is equal to the velocity multiplied by the crosssectional area of the flowing liquid. The continuity law can be expressed : Q = v 1 A 1 = v 2 A 2 where Q = volumetric flow rate, cm 3 /s (in3/sec); v = velocity as before; A = cross sectional area of the liquid, cm 2 and the subscripts refer to any two points in the flow system. Thus, an increase in area results in a decrease in velocity, and vice versa. Equations indicate that the sprue should be tapered. As the metal accelerates during its descent into the sprue opening, the crosssectional area of the channel must be reduced; otherwise, as the velocity of the flowing metal increases toward the base of the sprue, air can be aspirated into the liquid and conducted into the mold cavity. To prevent this condition, the sprue is designed with a taper, so that the volume flow rate va is the same at the top and bottom of the sprue.

6 Schematic showing the advantages of a tapered sprue over a straight-sided sprue. (a) Natural flow of a free-falling liquid. (b) Air aspiration induced by liquid flow in a straight-sided sprue. (c) Liquid flow in a tapered sprue. Assuming that the runner from the sprue base to the mold cavity is horizontal (and therefore the head h is the same as at the sprue base), then the volume rate of flow through the gate and into the mold cavity remains equal to va at the base. Accordingly, we can estimate the time required to fill a mold cavity of volume V as MFT = V Q Where TMF=mold filling time, s (sec);v=volume of mold cavity, cm 3 and Q=volume flow rate, as before. The mold filling time computed by Eq. (6) must be considered a minimum time. This is because the analysis ignores friction losses and possible constriction of flow in the gating system; thus, the mold filling time will be longer than what is given by Eq. (6). EX2 A mold sprue is 20 cm long, and the cross-sectional area at its base is 2.5 cm2. The sprue feeds a horizontal runner leading into a mold cavity whose volume is 1560 cm 3. Determine: (a) velocity of the molten metal at the base of the sprue, (b) volume rate of flow, (c) time to fill the mold. (a)the velocity of the flowing metal at the base of the Sprue is given by Eq. (4): V= 2(981)(20) = cm/s (b) The volumetric flow rate is Q =( 2.5 cm 2 )(198.1 cm/s)= 495 cm 2 /s (c) Time required to fill a mold cavity of 100 in3 at this flow rate is TMF = 1560/495 = 3.2s

7 FLUIDITY The molten metal flow characteristics are often described by the term fluidity, a measure of the capability of a metal to flow into and fill the mold before freezing. Fluidity is the inverse of viscosity as viscosity increases, fluidity decreases. Standard testing methods are available to assess fluidity, including the spiral mold test shown in Figure in which fluidity is indicated by the length of the solidified metal in the spiral channel. A longer cast spiral means greater fluidity of the molten metal. Factors affecting fluidity include 1. pouring temperature relative to melting point, 2. metal composition 3. viscosity of the liquid metal 4. heat transfer to the surroundings. A higher pouring temperature relative to the freezing point of the metal increases the time it remains in the liquid state, allowing it to flow further before freezing. This tends to aggravate certain casting problems such as oxide formation, gas porosity, and penetration of liquid metal into the interstitial spaces between the grains of sand forming the mold. This last problem causes the surface of the casting to contain imbedded sand particles, thus making it rougher and more abrasive than normal. Composition also affects fluidity, particularly with respect to the metal s solidification mechanism. The best fluidity is obtained by metals that freeze at a constant temperature (e.g., pure metals and eutectic alloys). When solidification occurs over a temperature range (most alloys are in this category), the partially solidified portion interferes with the flow of the liquid portion, thereby reducing fluidity. In addition to the freezing mechanism, metal composition also determines heat of fusion the amount of heat required to solidify the metal from the liquid state.

8 A higher heat of fusion tends to increase the measured fluidity in casting. Fluidity Test

9 Problems in Heating and Pouring 10.1 A disk 40 cm in diameter and 5 cm thick is to be cast of pure aluminum in an open-mold casting operation. The melting temperature of aluminum = 660 C, and the pouring temperature will be 800 C. Assume that the amount of aluminum heated will be 5% more than what is needed to fill the mold cavity. Compute the amount of heat that must be added to the metal to heat it to the pouring temperature, starting from a room temperature of 25 C. The heat of fusion of aluminum = J/g. Other properties can be obtained from Tables 4.1 and 4.2 in the text. Assume the specific heat has the same value for solid and molten aluminum A sufficient amount of pure copper is to be heated for casting a large plate in an open mold. The plate has dimensions: length= 20 in, width = 10 in, and thickness 3 in. Compute the amount of heat that must be added to the metal to heat it to a temperature of 2150 F for pouring. Assume that the amount of metal heated will be 10% more than what is needed to fill the mold cavity. Properties of the metal are: density=0.324 lbm/in 3, melting point = 1981 F, specific heat of the metal = Btu/lbm F in the solid state and Btu/lbm F in the liquid state, and heat of fusion =80 Btu/lbm The down sprue leading into the runner of a certain mold has a length = 175 mm. The cross-sectional area at the base of the sprue is 400mm 2. The mold cavity has a volume ¼ 0.001m 3. Determine (a) the velocity of the molten metal flowing through the base of the downsprue, (b) the volume rate of flow, and (c) the time required to fill the mold cavity A mold has a down sprue of length = 6.0 in. The

10 cross-sectional area at the bottom of the sprue is 0.5 in 2. The sprue leads into a horizontal runner which feeds the mold cavity, whose volume = 75 in 3. Determine (a) the velocity of the molten metal flowing through the base of the down sprue, (b) the volume rate of flow, and (c) the time required to fill the mold cavity The flow rate of liquid metal into the downsprue of a mold = 1 L/s. The cross-sectional area at the top of the sprue =800 mm 2, and its length =175 mm. What area should be used at the base of the sprue to avoid aspiration of the molten metal? The volume rate of flow of molten metal into the Down sprue from the pouring cup is 50 in 3 /sec. At the top where the pouring cup leads into the downsprue, the cross-sectional area=1.0 in 2.Determine what the area should be at the bottom of the sprue if its length =8.0 in. It is desired to maintain a constant flow rate, top and bottom, in order to avoid aspiration of the liquid metal Molten metal can be poured into the pouring cup of a sand mold at a steady rate of 1000 cm 3 /s. The molten metal overflows the pouring cup and flows into the downsprue. The cross-section of the sprue is round, with a diameter at the top= 3.4 cm. If the sprue is 25cm long, determine the proper diameter at its base so as to maintain the same volume flow rate During pouring into a sand mold, the molten metal can be poured into the downsprue at a constant flow rate during the time it takes to fill the mold. At the end of pouring the sprue is filled and there is negligible metal in the pouring cup. The downsprue is 6.0 in long. Its cross-sectional area at the top¼0.8 in2 and at the base=0.6 in 2.The cross-sectional area of the runner leading from the sprue also = 0.6 in 2, and it is 8.0 in long before leading into the mold cavity, whose volume=65 in 3. The volume of the riser located along the runner near the mold cavity= 25 in 3. It takes a total of 3.0 sec to fill the entire mold

11 (including cavity, riser, runner, and sprue. This is more than the theoretical time required, indicating a loss of velocity due to friction in the sprue and runner. Find (a) the theoretical down sprue velocity and flow rate at the base of the Mold (b) the total volume of the mold; (c) the actual velocity and flow rate at the base of the sprue; (d) the loss of head in the gating system due to friction.

### Prediction of Solidification Time: Chvorinov's Rule.

Prediction of Solidification Time: Chvorinov's Rule. The amount of heat that must be removed from a casting to cause it to solidify is directly proportional to the amount of superheating and the amount

### Production of ductile iron castings without feeders

Production of ductile iron castings without feeders Possibilities of producing ductile iron castings in green sand mould without feeders by means of "ingate" feeding and control of the graphite precipitation

### Fundamentals of Metal Casting

Chapter 10 Fundamentals of Metal Casting QUALITATIVE PROBLEMS 10.15 Describe the stages involved in the contraction of metals during casting. The stages involved in the contraction of metals during casting

### Design of Cast Parts Avoid sharp corners, angles & fillets They act as stress raisers Select fillet radii to reduce stress concentrations and ensure p

Metal Casting Design, Materials, Economics Text Reference: Manufacturing Engineering and Technology, Kalpakjian & Schmid, 6/e, 2010 Chapter 12 Design of Cast Parts Avoid sharp corners, angles & fillets

### UNIT 47: Gating Design Wizard

UNIT 47: Gating Design Wizard The SOLIDCast Gating Design Wizard is an integrated function of the SOLIDCast system. The Gating Design Wizard allows you to size sprues, runners and gates for either horizontally-parted

### ME 333 Manufacturing Processes II

ME 333 Manufacturing Processes II Chapter 2 Foundry Processes Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana Introduction Some Terminology Foundry processes

### 3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?

ecture 18-22: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,

### MIT 2.810 Manufacturing Processes and Systems. Homework 6 Solutions. Casting. October 15, 2015. Figure 1: Casting defects

MIT 2.810 Manufacturing Processes and Systems Casting October 15, 2015 Problem 1. Casting defects. (a) Figure 1 shows various defects and discontinuities in cast products. Review each one and offer solutions

### Casting of Brake Disc and Impeller from Aluminium Scrap Using Silica Sand

Leonardo Electronic Journal of Practices and Technologies ISSN 1583-1078 Issue 10, January-June 2007 p. 145-150 Casting of Brake Disc and Impeller from Aluminium Scrap Using Silica Sand Department of Mechanical

### Chapter 28 Fluid Dynamics

Chapter 28 Fluid Dynamics 28.1 Ideal Fluids... 1 28.2 Velocity Vector Field... 1 28.3 Mass Continuity Equation... 3 28.4 Bernoulli s Principle... 4 28.5 Worked Examples: Bernoulli s Equation... 7 Example

### 5.6: Characteristic Physical Properties pg. 192

5.6: Characteristic Physical Properties pg. 192 Key Concepts: 1. Physical properties are characteristics that can be determined without changing the composition of the substance. 3. Pure substances have

### For Water to Move a driving force is needed

RECALL FIRST CLASS: Q K Head Difference Area Distance between Heads Q 0.01 cm 0.19 m 6cm 0.75cm 1 liter 86400sec 1.17 liter ~ 1 liter sec 0.63 m 1000cm 3 day day day constant head 0.4 m 0.1 m FINE SAND

### Module 1 : Conduction. Lecture 5 : 1D conduction example problems. 2D conduction

Module 1 : Conduction Lecture 5 : 1D conduction example problems. 2D conduction Objectives In this class: An example of optimization for insulation thickness is solved. The 1D conduction is considered

### This chapter describes how you can model solidification and melting in FLUENT. Information is organized into the following sections:

Chapter 21. Melting Modeling Solidification and This chapter describes how you can model solidification and melting in FLUENT. Information is organized into the following sections: Section 21.1: Overview

### Experiment 3 Pipe Friction

EML 316L Experiment 3 Pipe Friction Laboratory Manual Mechanical and Materials Engineering Department College of Engineering FLORIDA INTERNATIONAL UNIVERSITY Nomenclature Symbol Description Unit A cross-sectional

### Feeding & Risering Guidelines for Steel Castings

Feeding & Risering Guidelines for Steel Castings Steel Founders Society of America 2001 Index 1 Preface... 2 2 Risering basics and terminology... 4 3 Risering procedure... 10 4 Casting soundness in terms

### FLUID FLOW Introduction General Description

FLUID FLOW Introduction Fluid flow is an important part of many processes, including transporting materials from one point to another, mixing of materials, and chemical reactions. In this experiment, you

### DESIGN AND ANALYSIS OF GATING SYSTEM FOR SB-CNC TAIL STOCK BASE CASTING

DESIGN AND ANALYSIS OF GATING SYSTEM FOR SB-CNC TAIL STOCK BASE CASTING Rohith K R 1, Rahul R 2, Liroy Oppan 3, Sheryl John 4, Amal Mohan 5, Renjith Venugopal 6, Susruthan A S 7 Bessy Paul 8, Saravanan

### Analysis and Optimization of Investment Castings to Reduce Defects and Increase Yield

Analysis and Optimization of Investment Castings to Reduce Defects and Increase Yield Arunkumar P 1, Anand.S.Deshpande 2, Sangam Gunjati 3 1 Associate Professor, Mechanical Engineering, KLS Gogte Institute

### Simulation of Centrifugal Casting via STAR-Cast. Santhanu Jana, Access e.v., Aachen

Simulation of Centrifugal Casting via STAR-Cast Santhanu Jana, Access e.v., Aachen Talk overview Centrifugal casting STAR-Cast s modelling basis Motivation for centrifugal investment casting Centrifugal

### FLUID DYNAMICS. Intrinsic properties of fluids. Fluids behavior under various conditions

FLUID DYNAMICS Intrinsic properties of fluids Fluids behavior under various conditions Methods by which we can manipulate and utilize the fluids to produce desired results TYPES OF FLUID FLOW Laminar or

### CENTRIFUGAL CASTING. Email: amitjoshi@iitb.ac.in amitjoshi1000@yahoo.ca

CENTRIFUGAL CASTING Amit M Joshi (B.Engg. Mechanical, A.M.I.Prod.E, A.I.E) Dept. of Metallurgical Engg. & Material Science, Indian Institute of Technology Bombay, India. Email: amitjoshi@iitb.ac.in amitjoshi1000@yahoo.ca

### 1.2 CASTING PROCESSES EXPENDABLE MOLD CASTING. Sand Casting

Valery Marinov, Manufacturing Technology Metal Casting 5 1.2 CASTING PROCESSES Sand Casting EXPENDABLE MOLD CASTING In expendable mold casting, the mold is destroyed to remove the casting and a new mold

### Plastic Injection Molds

Training Objective After watching the program and reviewing this printed material, the viewer will become familiar with the variety, design, and productive use of plastic injection molds. Mold components

### Applied Fluid Mechanics

Applied Fluid Mechanics 1. The Nature of Fluid and the Study of Fluid Mechanics 2. Viscosity of Fluid 3. Pressure Measurement 4. Forces Due to Static Fluid 5. Buoyancy and Stability 7. General Energy Equation

### CHAPTER 2 INJECTION MOULDING PROCESS

CHAPTER 2 INJECTION MOULDING PROCESS Injection moulding is the most widely used polymeric fabrication process. It evolved from metal die casting, however, unlike molten metals, polymer melts have a high

### The Most General Applications of Bernoulli s Equation

The Most General Applications of Bernoulli s Equation Bởi: OpenStaxCollege Torricelli s Theorem [link] shows water gushing from a large tube through a dam. What is its speed as it emerges? Interestingly,

### XI / PHYSICS FLUIDS IN MOTION 11/PA

Viscosity It is the property of a liquid due to which it flows in the form of layers and each layer opposes the motion of its adjacent layer. Cause of viscosity Consider two neighboring liquid layers A

### Solid shape molding is not desired in injection molding due to following reasons.

PLASTICS PART DESIGN and MOULDABILITY Injection molding is popular manufacturing method because of its high-speed production capability. Performance of plastics part is limited by its properties which

### Fe-C Phase Diagram Introduction

FUNDAMENTALS OF METAL CASTING 0. Phase Diagram 1. Overview. Heating & Pouring 3. Solidification and Cooling 0. Alloys and Phase Diagram Pure Metals Alloys Solid solutions Substitutional Solid Solution

### MODELING OF AN AEROSPACE SAND CASTING PROCESS. A Thesis: submitted to the Faculty. of the WORCESTER POLYTECHNIC INSTITUTE

MODELING OF AN AEROSPACE SAND CASTING PROCESS A Thesis: submitted to the Faculty of the WORCESTER POLYTECHNIC INSTITUTE in partial fulfillment of the requirements for the Degree of Master of Science In

### Multiphysics CAE Simulations of Casting Process for the First Time Right Product Development

Multiphysics CAE Simulations of Casting Process for the First Time Right Product Development Mir Mehdi Hussain *, Ramanathan SV, and Raj C Thiagarajan *Corresponding Author ATOA Scientific Technologies

### Chapter 13 Fluids. Copyright 2009 Pearson Education, Inc.

Chapter 13 Fluids 13-1 Phases of Matter The three common phases of matter are solid, liquid, and gas. A solid has a definite shape and size. A liquid has a fixed volume but can be any shape. A gas can

### The soot and scale problems

Dr. Albrecht Kaupp Page 1 The soot and scale problems Issue Soot and scale do not only increase energy consumption but are as well a major cause of tube failure. Learning Objectives Understanding the implications

### Understanding Plastics Engineering Calculations

Natti S. Rao Nick R. Schott Understanding Plastics Engineering Calculations Hands-on Examples and Case Studies Sample Pages from Chapters 4 and 6 ISBNs 978--56990-509-8-56990-509-6 HANSER Hanser Publishers,

### Defect formation in cast iron

Defect formation in cast iron School of Engineering Jönköping University Sweden Tammerfors, Finland, November 8, 2012 Introduction Casting Mould cavity Melting process Pouring Solidification Mould removal

### GLOBAL MANUFACTURING. ARAUJO, Anna Carla AUG, 2015 Mechanical Engineering Department POLI/COPPE/UFRJ

GLOBAL MANUFACTURING ARAUJO, Anna Carla AUG, 2015 Mechanical Engineering Department POLI/COPPE/UFRJ Workpiece Presentation Powder Metallurgy and Additive Manufacturing [#7] Powder Metallurgy PM parts can

### Plastic Injection Molding

Training Objective After watching this video and reviewing the printed material, the student/trainee will understand the principles and physical operations of the plastic injection molding process. An

### RESEARCH PROJECT. High Pressure Die Casting Defects and Simulation Process by Computer Added Engineering (CAE)

RESEARCH PROJECT High Pressure Die Casting Defects and Simulation Process by Computer Added Engineering (CAE) ME8109 CASTING AND SOLIDIFICATION OF MATERIALS Presented by: Irshad Ali (Student # 500482510)

### MANUFACTURING PROCESSES

MANUFACTURING PROCESSES - AMEM 201 Lecture 3: Casting Technology DR. SOTIRIS L. OMIROU Manufacturing Processes - classification - CASTING FORMING Casting A manufacturing process that pours a liquid material

### An Analysis of Heat Conduction with Phase Change during the Solidification of Copper

An Analysis of Heat Conduction with Phase Change during the Solidification of Copper J. Michalski and E. Gutierrez-Miravete *2 1 Hamilton Sundstrand, 2 Rensselaer at Hartford *Corresponding author: 275

### Development of NG Fueled Steel Cutting Torch for Industrial Application.

Development of NG Fueled Steel Cutting Torch for Industrial Application. Hyun-Seok You, Korea Gas Cooperation Research & Development Div. Hyun-Chan Lee, Korea Gas Cooperation Research & Development Div.

### PSS 17.1: The Bermuda Triangle

Assignment 6 Consider 6.0 g of helium at 40_C in the form of a cube 40 cm. on each side. Suppose 2000 J of energy are transferred to this gas. (i) Determine the final pressure if the process is at constant

### oil liquid water water liquid Answer, Key Homework 2 David McIntyre 1

Answer, Key Homework 2 David McIntyre 1 This print-out should have 14 questions, check that it is complete. Multiple-choice questions may continue on the next column or page: find all choices before making

### 2.0 BASIC CONCEPTS OF OPEN CHANNEL FLOW MEASUREMENT

2.0 BASIC CONCEPTS OF OPEN CHANNEL FLOW MEASUREMENT Open channel flow is defined as flow in any channel where the liquid flows with a free surface. Open channel flow is not under pressure; gravity is the

### Swissmetro travels at high speeds through a tunnel at low pressure. It will therefore undergo friction that can be due to:

I. OBJECTIVE OF THE EXPERIMENT. Swissmetro travels at high speeds through a tunnel at low pressure. It will therefore undergo friction that can be due to: 1) Viscosity of gas (cf. "Viscosity of gas" experiment)

### Heat Transfer Prof. Dr. Ale Kumar Ghosal Department of Chemical Engineering Indian Institute of Technology, Guwahati

Heat Transfer Prof. Dr. Ale Kumar Ghosal Department of Chemical Engineering Indian Institute of Technology, Guwahati Module No. # 04 Convective Heat Transfer Lecture No. # 03 Heat Transfer Correlation

### Casting. Training Objective

Training Objective After watching the program and reviewing this printed material, the viewer will learn the essentials of the various metal casting processes used in industry today. The basic principles

### STUDY OF PROCESS PARAMETERS OF GRAVITY DIE CASTING DEFECTS

International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 2, March-April 2016, pp. 208 211, Article ID: IJMET_07_02_023 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=2

### Open channel flow Basic principle

Open channel flow Basic principle INTRODUCTION Flow in rivers, irrigation canals, drainage ditches and aqueducts are some examples for open channel flow. These flows occur with a free surface and the pressure

### THERMOCHEMISTRY & DEFINITIONS

THERMOCHEMISTRY & DEFINITIONS Thermochemistry is the study of the study of relationships between chemistry and energy. All chemical changes and many physical changes involve exchange of energy with the

### 5. DIMENSIONS, TOLERANCES AND SURFACE. 5.1 Dimension, Tolerances and Related Attributes 5.2 Surfaces 5.3 Effect of Manufacturing Processes

5. DIMENSIONS, TOLERANCES AND SURFACE 5.1 Dimension, Tolerances and Related Attributes 5.2 Surfaces 5.3 Effect of Manufacturing Processes Introduction Dimensions the sizes and geometric features of a component

### Thermal Analysis TGA / DTA. Linda Fröberg

Thermal Analysis TGA / DTA Linda Fröberg Outline Definitions What is thermal analysis? Instrumentation & origin of the TGA-DTA signal. TGA DTA Basics and applications Phase diagrams & Thermal analysis

### Chapter 12 - Liquids and Solids

Chapter 12 - Liquids and Solids 12-1 Liquids I. Properties of Liquids and the Kinetic Molecular Theory A. Fluids 1. Substances that can flow and therefore take the shape of their container B. Relative

### Boundary Conditions in Fluid Mechanics

Boundary Conditions in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University The governing equations for the velocity and pressure fields are partial

### A NOVEL SINTERING-DISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS

Scripta mater. 44 (2001) 105 110 www.elsevier.com/locate/scriptamat A NOVEL SINTERING-DISSOLUTION PROCESS FOR MANUFACTURING Al FOAMS Y.Y. Zhao and D.X. Sun Materials Science and Engineering, Department

### The Most General Applications of Bernoulli's Equation

OpenStax-CNX module: m42208 1 The Most General Applications of Bernoulli's Equation OpenStax College This work is produced by OpenStax-CNX and licensed under the Creative Commons Attribution License 3.0

### Sand Casting of Metals

Sand Casting of Metals Elizabeth Merten Department of Materials Science & Engineering University of Washington Seattle, WA 98195 emerten@u.washington.edu Copyright Edmonds Community College 2012 This material

### CEE 370 Fall 2015. Laboratory #3 Open Channel Flow

CEE 70 Fall 015 Laboratory # Open Channel Flow Objective: The objective of this experiment is to measure the flow of fluid through open channels using a V-notch weir and a hydraulic jump. Introduction:

### Ablation of Hybrid Metal Matrix Composites

Paper 11-057.pdf, Page 1 of 7 Copyright 2011 American Foundry Society Ablation of Hybrid Metal Matrix Composites D. Weiss Eck Industries, Manitowoc, WI J. Grassi Alotech LLC Ltd., Brooklyn, OH B. Schultz,

### Casting Defects - Blow holes:

Casting Defects - Blow holes: It is only through extensive research that it is possible to share this type of information. One needs to understand that in the age of the internet all of the information

### A LAMINAR FLOW ELEMENT WITH A LINEAR PRESSURE DROP VERSUS VOLUMETRIC FLOW. 1998 ASME Fluids Engineering Division Summer Meeting

TELEDYNE HASTINGS TECHNICAL PAPERS INSTRUMENTS A LAMINAR FLOW ELEMENT WITH A LINEAR PRESSURE DROP VERSUS VOLUMETRIC FLOW Proceedings of FEDSM 98: June -5, 998, Washington, DC FEDSM98 49 ABSTRACT The pressure

### FEATURES AND BENEFITS OF DIFFERENT PLATINUM ALLOYS. Kris Vaithinathan and Richard Lanam Engelhard Corporation

FEATURES AND BENEFITS OF DIFFERENT PLATINUM ALLOYS Kris Vaithinathan and Richard Lanam Engelhard Corporation Introduction There has been a significant increase in the world wide use of platinum for jewelry

### Welding Engineering Prof. Dr. D. K. Dwivedi Department of Mechanical and Industrial Engineering Indian Institute of Technology, Roorkee

Welding Engineering Prof. Dr. D. K. Dwivedi Department of Mechanical and Industrial Engineering Indian Institute of Technology, Roorkee Module - 4 Arc Welding Processes Lecture - 2 SMAW - II So, in this

ALUMINUM CASTING COMPARISON CHARTS A Qualitative Comparison of Several Competing Processes for the Production of Aluminum Castings The following charts are intended to provide a relative guide to compare

### A model of heat transfer in metal foaming

A model of heat transfer in metal foaming B. Chinè 1,2, V. Mussi 2, M. Monno 3, A Rossi 2 1 Instituto Tecnológico de Costa Rica, Costa Rica; 2 Laboratorio MUSP, Macchine Utensili e Sistemi di Produzione,

### Module 2 : Convection. Lecture 20a : Illustrative examples

Module 2 : Convection Lecture 20a : Illustrative examples Objectives In this class: Examples will be taken where the concepts discussed for heat transfer for tubular geometries in earlier classes will

### Composition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)

10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature

### UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121. Spring Semester 2008 Professor R.

UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above

### Development of Mathematical Equation for Fraction of Solid in AlSi7Mg Alloy Solidification Simulation

Journal of Minerals & Materials Characterization & Engineering, Vol. 7, No.1, pp 71-8, 007 jmmce.org Printed in the USA. All rights reserved Development of Mathematical Equation for Fraction of Solid in

### FLUID FLOW STREAMLINE LAMINAR FLOW TURBULENT FLOW REYNOLDS NUMBER

VISUAL PHYSICS School of Physics University of Sydney Australia FLUID FLOW STREAMLINE LAMINAR FLOW TURBULENT FLOW REYNOLDS NUMBER? What type of fluid flow is observed? The above pictures show how the effect

### What is a mold? Casting. Die casting. Injection Molding Machine. Injection Molding. 2.008 Design & Manufacturing II. Spring 2004

2.008 Design & Manufacturing II What is a mold? From Webster: a cavity in which a substance is shaped: as (1) : a matrix for casting metal (2) : a form in which food is given a decorative shape Spring

### Module - 2 Advanced Metal Casting Processes Lecture - 2 Evaporative Pattern Casting Processes (EPC)

Advanced Manufacturing Processes Prof. Dr. Apurbba Kumar Sharma Department of Mechanical and Industrial Engineering Indian Institute of Technology, Roorkee Module - 2 Advanced Metal Casting Processes Lecture

### Lecture 33 continuous casting of steel. Keywords: continuous casting, tundish metallurgy, secondary cooling, defects in cast product

Contents Introduction How casting is done continuously Tundish Mold secondary cooling Heat transfer in continuous casting Product and casting defect Lecture 33 continuous casting of steel Keywords: continuous

### Assessment of Low-Temperature Fluxes

Assessment of Low-Temperature Fluxes The subject of this paper is the evaluation of the wetting balance as a technique for studying the flux activity of newly developed low-temperature solder paste fluxes.

### HEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi

HEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi 2 Rajesh Dudi 1 Scholar and 2 Assistant Professor,Department of Mechanical Engineering, OITM, Hisar (Haryana)

### Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen

Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen Tagung des Arbeitskreises Thermophysik, 4. 5.3.2010 Karlsruhe, Deutschland E. Kaschnitz Österreichisches Gießerei-Institut

### Laminar and Turbulent flow. Flow Sensors. Reynolds Number. Thermal flow Sensor. Flow and Flow rate. R = Mass Flow controllers

Flow and Flow rate. Laminar and Turbulent flow Laminar flow: smooth, orderly and regular Mechanical sensors have inertia, which can integrate out small variations due to turbulence Turbulent flow: chaotic

### Comparison of Three Ni-Hard I Alloys

Comparison of Three Ni-Hard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:

### Chemistry 13: States of Matter

Chemistry 13: States of Matter Name: Period: Date: Chemistry Content Standard: Gases and Their Properties The kinetic molecular theory describes the motion of atoms and molecules and explains the properties

### Fluid Mechanics Definitions

Definitions 9-1a1 Fluids Substances in either the liquid or gas phase Cannot support shear Density Mass per unit volume Specific Volume Specific Weight % " = lim g#m ( ' * = +g #V \$0& #V ) Specific Gravity

### UNIT 20: Output Criteria: Solidification Time

UNIT 20: Output Criteria: Solidification Time Solidification Time shows the time, in minutes, for each part of the casting to become COMPLETELY solid, i.e., to cool to the Solidus Point. Viewing a plot

### THE WAY TO SOMEWHERE. Sub-topics. Diffusion Diffusion processes in industry

THE WAY TO SOMEWHERE Sub-topics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation

### Kursus i Produktions- og materialeteknologi

Kursus i Produktions- og materialeteknologi Plastsprøjtestøbning / Injection Molding Basics Short history of plastics 1862 first synthetic plastic 1866 Celluloid 1891 Rayon 1907 Bakelite 1913 Cellophane

### Injection molding equipment

Injection Molding Process Injection molding equipment Classification of injection molding machines 1. The injection molding machine processing ability style clamping force(kn) theoretical injection volume(cm3)

### TIE-31: Mechanical and thermal properties of optical glass

PAGE 1/10 1 Density The density of optical glass varies from 239 for N-BK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density

### DEVELOPMENT OF A METHOD FOR THE PRODUCTION OF ALUMINUM METAL FOAMS

International Journal Metallurgical & Materials Science and Engineering (IJMMSE) ISSN(P): 2278-2516; ISSN(E): 2278-2524 Vol. 4, Issue 1, Feb 2014, 9-14 TJPRC Pvt. Ltd. DEVELOPMENT OF A METHOD FOR THE PRODUCTION

### TILT POUR TRIALS AND ANALYSIS. Matrix Metals Keokuk Facility (Keokuk Steel Castings) Keokuk, Iowa 52632

TILT POUR TRIALS AND ANALYSIS Bob Bryant 1, Kent D. Carlson 2, Shouzhu Ou 2, Christoph Beckermann 2 1 Matrix Metals Keokuk Facility (Keokuk Steel Castings) Keokuk, Iowa 52632 2 Department of Mechanical

### Differential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation

Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of

### Introduction to Metallography

Introduction to Metallography Metallography has been described as both a science and an art. Traditionally, metallography has been the study of the microscopic structure of metals and alloys using optical

### Experiment (13): Flow channel

Introduction: An open channel is a duct in which the liquid flows with a free surface exposed to atmospheric pressure. Along the length of the duct, the pressure at the surface is therefore constant and

### DRY SAND ABRASIVE WEAR BEHAVIOR OF CHILL CAST ALUMINUM BORON CARBIDE COMPOSITES

DRY SAND ABRASIVE WEAR BEHAVIOR OF CHILL CAST ALUMINUM BORON CARBIDE COMPOSITES K. V. Sreenivas Rao 1, Sanman S. 1, Sanjeevamurthy 1 and T. P. Bharathesh 2 1 Department of Mechanical Engineering, Siddaganga

### p atmospheric Statics : Pressure Hydrostatic Pressure: linear change in pressure with depth Measure depth, h, from free surface Pressure Head p gh

IVE1400: n Introduction to Fluid Mechanics Statics : Pressure : Statics r P Sleigh: P..Sleigh@leeds.ac.uk r J Noakes:.J.Noakes@leeds.ac.uk January 008 Module web site: www.efm.leeds.ac.uk/ive/fluidslevel1

### Specific Heat Capacity and Latent Heat Questions A2 Physics

1. An electrical heater is used to heat a 1.0 kg block of metal, which is well lagged. The table shows how the temperature of the block increased with time. temp/ C 20.1 23.0 26.9 30.0 33.1 36.9 time/s

### Fluids and Solids: Fundamentals

Fluids and Solids: Fundamentals We normally recognize three states of matter: solid; liquid and gas. However, liquid and gas are both fluids: in contrast to solids they lack the ability to resist deformation.

### (a) Calculate the voidage (volume fraction occupied by voids) of the bed.

SOLUTIONS TO CAPTER 6: FLOW TROUG A PACKED BED OF PARTICLES EXERCISE 6.1: A packed bed of solid particles of density 500 kg/m 3, occupies a depth of 1 m in a vessel of cross-sectional area 0.04 m. The

### Conservation of Energy Physics Lab VI

Conservation of Energy Physics Lab VI Objective This lab experiment explores the principle of energy conservation. You will analyze the final speed of an air track glider pulled along an air track by a

### FILTRATION. Introduction. Batch Filtration (Small Scale) Controlling parameters: Pressure drop, time for filtration, concentration of slurry

FILTRATION Introduction Separation of solids from liquids is a common operation that requires empirical data to make predictions of performance. These data are usually obtained from experiments performed

### I SOIL WATER POTENTIAL

I SOIL WATER POTENTIAL 1.1. Introduction Soil water content is not sufficient to specify the entire status of water in soil. For example, if soils with a same water content but with different particle

### Welcome to the World of Chemistry

Welcome to the World of Chemistry The Language of Chemistry CHEMICAL ELEMENTS - pure substances that cannot be decomposed by ordinary means to other substances. Aluminum Bromine Sodium The Language of